# Understanding Hardness Testing: A Complete Guide

Ever wondered why diamonds are so hard? In this article, we’ll explore the fascinating world of material hardness, from talc to diamond. You’ll learn how different tests, like Brinell, Rockwell, and Vickers, measure this crucial property, and why it matters in engineering. Get ready to uncover the secrets behind the strength of materials!

## 1. Overview

Hardness: the ability to resist local indentation deformation or scratch fracture.

Two kinds of Mohs hardness sequence tables

## 2. Brinell hardness

### (1) Principle

To determine the Brinell hardness of a metal material, apply a certain load F with a spherical indenter of diameter D onto its surface and maintain it for a specific duration. This process will result in the formation of a spherical indentation, and the load value per unit area of the indentation is considered as the Brinell hardness of the metal material.

Measuring indentation diameter

Indenter material：

• Hard alloy ball (HBW) HB=450~650
• Hardened steel ball (HBS) HB<450

### (2) Representation method

For example: 280HBS10/3000/30
1kgf=9.81N

• 280 – Hardness value
• HBS – Hardness symbol
• 10 – Diameter of steel ball mm
• 3000 – Load size kgf
• 30 – Load holding time s

General conditions: 10mm steel ball diameter; 3000kg load; 10s pressure holding time, namely HB280

### (4) Selection of F and D (principle of geometric similarity of indentation)

When measuring Brinell hardness with indenters of different diameters and loads of different sizes, the principle of geometric similarity must be met to obtain the same HB value, that is, the opening angleφ of the indentation is equal.

Method: The same HB shall be measured for samples with the same material but different thickness, or materials with different hardness and softness.

When selecting D and F, F/D2 shall be the same.

Principle of geometrical similarity of indentation:

It can be seen that as long as F/D remains constant, HB only depends on the pressing angle φ.

F/D2 ratio: 30,15,10,5,2.5,1.25,1

According to the engineering regulations, the ratio of F/D2 is 30, 10 and 2.5, which are selected according to the material hardness and sample thickness.

See various standards and test specifications for details.

Fig. 1-21 Application of similarity principle

Selection Table of Brinell Hardness Test P/D2

The experiment shows that HB is stable and comparable when 0.25D<d<0.5D.

If it has influence on the test, it shall be carried out in strict accordance with the regulations, generally 10s and 30s.

### (6) Characteristics and Application of Brinell Hardness

This method is well-suited for coarse or heterogeneous materials due to its large indentation area and high measurement accuracy. However, due to the large indentation size, inspection of finished products can be challenging.

It is primarily utilized for inspecting raw materials, and the indenter material is limited to softer materials (HB450~650). Additionally, the efficiency of indentation measurement is relatively low.

## 3. Rockwell hardness

Indentation depth can be used to reflect the hardness of materials.

To adapt to different soft and hard materials, many grades of hardness testers use different indenters and loads.

One common grade is C, HRC, which uses a 150kgf total load and a 120° diamond cone indenter that is loaded twice.

First, an initial load of P1=10kgf is applied to ensure proper contact between the indenter and the material surface. Then, the main load of P2=140kgf is added.

After removing P2, the depth of the indentation is measured and used to determine the hardness of the material.

Fig. 3-17 Schematic Diagram of the Principle and Test Process of Rockwell Hardness Test

Indenter: 120 diamond cone or hardened steel ball

Rockwell hardness definition:

0.002mm residual indentation depth is a Rockwell hardness unit.

K – constant, 130 for steel ball indenter and 100 for diamond indenter

Table 3-6 Test Specification and Application of Rockwell Hardness

Characteristics and Application of Rockwell Hardness

(1) This method allows for direct reading of the hardness value and is highly efficient, making it suitable for batch inspection.

(2) The indentation is small and generally considered “nondestructive,” making it suitable for inspecting finished products.

(3) However, the small indentation size can result in poor representativeness and therefore is not suitable for coarse or non-uniform materials.

(4) The Rockwell hardness test is divided into various scales, each with a wide range of applications.

(5) It is important to note that Rockwell hardness values obtained from different scales are not comparable.

## 4. Vickers hardness

### 1. Principle

Press a diamond pyramid into the metal surface with a certain load F to form a pyramid indentation.

The load value on the unit indentation area is the Vickers hardness of the metal material.

When the unit of test force F is kgf:

When the unit of test force F is N:

Indenter material: diamond pyramid with an included angle of 136 °

### 2. Representation method

For example: 270HV30/20, if the holding time is 10-15s, it can be recorded as 270HV

• 270 – Hardness value
• 30 – Load size kgf
• 20 – Load holding time s

### 3. Microhardness

Indicated by Hm, it can be used to test the hardness of single grain or phase.

Characteristics and Application of Vickers Hardness

(1) The geometrical shape of the indentation is always similar, while the load can be varied.

(2) The corner cone indentation contour is distinct, resulting in high measurement accuracy.

(3) The diamond indenter has a broad range of applications and can provide consistent hardness scales for various materials.

(4) The efficiency of indentation measurement is low, making it unsuitable for on-site batch inspection.

(5) The indentation is small and not appropriate for coarse or heterogeneous materials.

However, metallographic specimens can be used to measure the hardness or hardness distribution of various phases.

## 5. Improvement of hardness strength relationship and test method

### (1) Hardness test characteristics

① The stress state is very soft (α>2), which is widely applicable;

Hardness of some materials

Covalent bond ≥ ionic bond>metal bond>hydrogen bond>Van’s bond

② The method is simple, nondestructive and suitable for field inspection;

③ The physical meaning is not clear, and it is difficult to design quantitatively.

### (2) Relationship between hardness and strength

σb≈KH

Steel: K=0.33~0.36

Copper alloy, stainless steel, etc.: K=0.4~0.55

Relationship between hardness and strength of annealed metals

Note: Unit of hardness!

### (3) Nano indentation test

During the loading process, elastic deformation first occurs on the surface of the specimen. As the load increases, plastic deformation gradually appears and also increases.

The unloading process is primarily the recovery of elastic deformation, while the plastic deformation ultimately causes an indentation to form on the sample surface.

Load displacement curve of nano indentation

Principle of nano indentation test

• H – Nano hardness;
• S – Contact stiffness;
• A – Contact area;
• β – Constants related to the geometry of the indenter;
• Er – equivalent modulus

There are important differences between nano hardness and traditional hardness:

First of all, the two definitions are different.

Nanohardness: the instantaneous force borne by a unit area on the projection of the surface area of the base indentation during the indentation process of the sample, which is a measure of the sample’s ability to withstand the contact load;

Vickers hardness is defined as the average force per unit area on the surface area of the indentation retained after the unloading of the indenter, which reflects the ability of the specimen to resist linear residual deformation.

In the process of measuring hardness, if plastic deformation dominates the process, the results of the two definitions are similar. However, if the process is dominated by elastic deformation, the results will differ.

In pure elastic contact, the residual contact area is very small. Therefore, the traditional definition of hardness will yield an infinite value, making it impossible to obtain the true hardness value of the sample.

Furthermore, the measurement ranges of the two methods are different. Traditional hardness measurement is only applicable to large-sized samples, not only due to limitations of the measuring instrument, but also because the residual indentation cannot accurately reflect the true hardness of the sample at the micro- and nano-scales.

New measurement techniques and calculation methods are used for nano hardness measurement, which can more accurately reflect the hardness characteristics of the sample at the micro- and nano-scales.

The key difference between the two methods is the calculation of indentation area. Nano hardness measurement involves measuring the indentation depth and then calculating the contact area using an empirical formula, whereas traditional hardness measurement involves obtaining the surface area of the indentation from photos taken after unloading.

### (4) Nanoindentation test method

The basic components of a nano hardness tester can be divided into several parts, including the control system, moving coil system, loading system, and indenter.

Diamond indenters, which are typically triangular cones or four-edge dimensions, are commonly used.

During the test, initial parameters are inputted first, and the subsequent detection process is fully automated by the microcomputer.

Manipulation of the loading system and the action of the indenter can be achieved by changing the current in the moving coil system.

Measurement and control of the indenter pressing load are carried out by the strain gauge, which also provides feedback to the moving coil system for closed-loop control, enabling completion of the test according to the input parameter settings.

Don't forget, sharing is caring! : )
Author

#### Shane

##### Founder of MachineMFG

As the founder of MachineMFG, I have dedicated over a decade of my career to the metalworking industry. My extensive experience has allowed me to become an expert in the fields of sheet metal fabrication, machining, mechanical engineering, and machine tools for metals. I am constantly thinking, reading, and writing about these subjects, constantly striving to stay at the forefront of my field. Let my knowledge and expertise be an asset to your business.

#### Punching Force Calculator & Formula (Online & Free)

Have you ever wondered how to ensure a successful metal stamping project? In this blog post, we'll dive into the critical factors that can make or break your stamping process.…

#### Sheet Metal Gauge Thickness Chart (Steel, Aluminum, Brass)

Have you ever wondered what those numbers on sheet metal mean? In this article, we'll dive into the world of sheet metal gauge and demystify this essential aspect of metalworking.…

#### Electric vs Hydraulic Press Brake – Which One is Right for Your Business?

I. Introduction With the increasing development of technology, modern sheet metal processing, especially the bending process, requires higher and higher standards. There are different technical requirements for equipment and processing…

#### Laser Cutting Thickness and Speed Chart (500W-30kW)

Curious about the capabilities of laser cutting? In this comprehensive guide, we'll dive into the world of laser cutting speeds and thicknesses for various metals. Our expert mechanical engineer will…

#### Z Purlin Weight Calculator & Chart (Online & Free)

Have you ever wondered about the hidden world of Z-purlins? In this captivating article, our expert mechanical engineer will guide you through the intricacies of calculating Z-purlin weight. Discover how…

#### H Beam Sizes and Weight Chart

Have you ever wondered about the hidden world of H-beam steel? In this captivating article, we'll unravel the mysteries behind these essential construction components. Our expert mechanical engineer will guide…

#### Chequered Plate Weight Calculator (Online & Free)

Have you ever wondered about the weight of those patterned steel plates you see every day? In this blog post, we'll dive into the fascinating world of checkered steel plates.…

#### K Factor Calculator for Sheet Metal Bending (Online & FREE)

Are you struggling to design accurate sheet metal parts? Unlock the secrets of the K-factor, a crucial concept in sheet metal fabrication. In this article, our expert mechanical engineer demystifies…

#### I Beam Weight Chart, Sizes & Online Calculator

Have you ever wondered how to select the perfect I-beam for your construction or manufacturing project? In this blog post, our expert mechanical engineer will guide you through the process…

#### Copper vs. Aluminum Cables: A Comprehensive Comparison

I. Advantages of Copper Core Cables over Aluminum Core Cables: 1. Low resistivity: The resistivity of aluminum core cables is about 1.68 times higher than that of copper core cables.…

#### How to Choose the Right Safety Valve: A Step-by-Step Guide

Due to the diversity of safety valves and the diversity and complexity of pressure systems, when selecting a safety valve, the impact of factors such as temperature, pressure, and medium…

#### Safety Valve Usage Tips: Enhance Your System’s Security

The researcher conducted a project on a hotel’s hot water system, which provides full-time supply with steam (0.3Mpa) as the heat source, water supply temperature of 60-55 degrees, using a…